Principles of Wool Fabric Finishing
Notes – Topic 15 – Principles of Wool Fabric Finishing
Notes – Topic 15 – Principles of Wool Fabric Finishing
15. Principles of Wool Fabric Finishing
Mike Pailthorpe and Errol Wood
On completion of this topic you should be able to:
· Explain the various types of dimensions change that can occur in fabrics
· Describe the finishing methods used to remove contaminants from greige state wool fabrics
· Outline the finishing methods used to stabilise the dimensions of wool fabrics
· Describe the methods used for drying wool fabrics
· Describe the finishing processes employed to modify the handle and appearance of wool fabrics
Key terms and concepts
Inspection, burling, mending, scouring, crabbing, carbonizing, milling, shrink proofing, bleaching, hydroextraction, scutching, drying, conditioning, raising, shearing, singeing, pressing, decatizing, perching.
Introduction to the topic
The objective of wool fabric finishing is to develop the desired properties in woollen and worsted fabrics that meet the specified end use requirements of consumers. Finishing is a sequence of dry and wet processes that is carried out in a logical order. There are four main objectives to be achieved from the finishing of wool fabrics.
· The removal, by scouring, of contaminants from the fabric. These contaminants may include lubricants and antistatic agents employed in yarn and fabric production, warp sizes and lubricants, machine oil stains, etc. In some cases the wool fabric may also contain vegetable matter (VM), in which case the process known as carbonising may be used to remove the VM
· The development of the required handle, softness, fullness, drape, etc.
· The control of the dimensional stability of the fabric, e.g. relaxation shrinkage, felting shrinkage, and hygral expansion
· The application of functional finishes, e.g. antistatic agents, flame-retardants, water-proofing agents, soil repellents, etc.
This lecture provides an overview of the principles of wool fabric finishing. The topic of wool fabric finishing is a very extensive one, and therefore can only be dealt with quite briefly here. While fabric dyeing can be regarded as a finishing process, this is discussed in Topic 13.
The general references for this topic are Rouette and Kitten (1991), Levene (1984), Brady (1997), De Boos (2003), Shaw and White (1984), Miles (2003) and Connell (2003). The Rouette and Kitten reference is a comprehensive book on the subject of wool fabric finishing.
Woven and knitted fabrics, taken straight from the loom or knitting machine, are known as greige (or grey) state fabrics. Such fabrics must be finished using wet and dry processes to produce high quality fabrics that are suitable for their intended use, e.g. suitings, knitwear, furnishing fabrics, etc.
The objectives of wet finishing of wool fabrics are firstly to remove contaminants from the wool by scouring and, if necessary, by carbonising. The latent stresses and strains the fabrics must then be relaxed, and the fabric set, in a process known as crabbing. Special qualities can then be developed in the wool fabrics by processes known as milling, shrink proofing, bleaching and dyeing. These so called wet finishing processes are grouped together, the aim being to minimise water consumption and to dry the fabric only once.
The so called dry finishing processes for wool fabrics follow on after hydroextraction and scutching, beginning with drying. One of the objectives in wool fabric finishing is to dry the fabric only once, to minimise energy usage.
Removal of contaminants
Greige-state fabrics (direct from the loom or knitting machine) are likely to contain contaminants that must be removed by a scouring (washing) process. These contaminants may include residual wool grease that was deliberately left on the wool after raw wool scouring, processing assistants (spinning lubricants, warp sizes, warp lubricants, antistatic agents, etc), adventitious soiling (machine oils, factory dust, lint, etc) and unfixed dyestuffs (from stock or yarn dyeing processes). If a greige-state fabric contains vegetable matter (VM), then it may be necessary to carbonize the fabric to destroy and remove the VM.
Improvement of dimensional stability
Greige-state wool fabrics have very poor dimensional stability, and great care must be taken in handling wool fabrics through the sequence of wet finishing processes. Depending upon fabric type, it may be necessary to stabilise the dimensions of the fabric before the scouring process, using a process known as crabbing. The decision to scour first, or crab first, is based upon the experience of the finisher. One of the risks in crabbing first is that one might set any stains in the wool fabric, making removal of the stains in subsequent scouring more difficult. Additional dimensional stability, together with lustre and handle, are achieved later in the finishing sequence by a process know as decatizing.
Wool fibres, like all animal fibres, have surface scales that give rise to the so called differential frictional effect (DFE). DFE, in combination with other fibre properties, can lead to felting shrinkage in wool fabrics. Finishers can make use of this property in a process known as milling (or fulling) to achieve consolidation of the fabric, increased fabric weight, reduced air permeability, etc. On the other hand, felting shrinkage can be detrimental to the performance of wool fabrics and the finisher must shrink-resist the fabrics. Shrink-resist processes may be degradative or additive. Degradative processes use chemicals, e.g. sodium hypochlorite, to chemically etch away the scales and hence reduce the DFE. Additive processes use polymers to either mask the scales or spot-weld the individual wool fibres together.
Whilst dyeing is not normally considered to be a part of the finishing process; dyeing can have a great influence on fabric quality. Wool fabric dyeing can be carried out in rope form or in open width form. Dyeing in rope form can lead to a degree of milling (consolidation) and may even completely change the character of the fabric. On the other hand, dyeing in open width may lead to flat setting of the fabric.
Once all the wet finishing processes have been completed, the fabric is dried. The first step in the drying sequence is the removal of liquid water from the fabric by mechanical means; usually by mangling or centrifuging. The second step is the removal of the remaining water using heat energy, usually in a stenter (or tenter). The stenter controls the dimensions of the fabric during drying by holding the selvedges of the fabric with tenter hooks or clamps.
After drying, a sequence of dry finishing processes is used to develop the fabric characteristics required by the end user of the fabric. Such processes include shearing, pressing and decatising to modify the fabric handle and appearance.
Depending upon the finish required, the wool fabrics may then either be shorn to remove surface fibres or brushed to create a pile of surface fibres. The brushed pile may be shorn to cut the pile fibres to a uniform height or to achieve a sculptured pattern.
The wool fabrics are then pressed using either flat, rotary or belt presses to achieve the desired appearance, lustre and handle characteristics. The effects of pressing are only temporary and hence the pressed fabric is then decatised to set the fabric. The set achieved in decatising should last through tailoring.
The decatised wool fabrics are relaxed by steaming, thereby reducing relaxation shrinkage in use. Finally, the finished fabrics are inspected for faults in a process known as perching.
15.2 Dimensional stability of wool fabrics
Changes of dimensions during use, and the caretreatments of textile materials, particularly textile materials containing natural fibres, can be a major defect and is often the cause of unserviceability and consumer complaint.
The types of dimensional change that can occur when wool fabrics are treated during processing, or in use, can be placed into five general groups:
(iv) felting, and
(v) hygral expansion due to changes in moisture content.
Relaxation shrinkage occurs when the stresses or strains imposed during the processing of the textile materials are relaxed in water (or water plus soap or detergent), without agitation. Relaxation shrinkage is what might be called the first stage of shrinkage. This form of shrinkage is common to all fibre types and fabric constructions and is non-reversible.
Special finishing processes relieve these strains, e.g. tensionless drying of knitted goods and the crabbing process applied to worsted fabrics.
The relaxation of residual strains in a fabric is frequently opposed by frictional constraints within the fabric brought about by fibre-fibre and yarn-yarn contacts. Further shrinkage; called consolidation shrinkage; can be brought about by gentle agitation in addition to simple soaking. This process is non-reversible.
In the case of knitted fabrics, consolidation shrinkage can occur with each washing. A bending of loops tends to occur due to the difference in twist at opposite sides of the loops. The strains are released upon washing and shrinkage occurs.
As can be seen from the data given in Table 15.1, when h